The first example of erbium triple-stranded helicates displaying SMM behaviour.
Gorczyński, Adam; Kubicki, Maciej; Pinkowicz, Dawid; Pełka, Robert; Patroniak, Violetta; Podgajny, Robert; Dalton transactions (Cambridge, England : 2003) 44 (2015) 16833–16839; doi:10.1039/c5dt02554k

data_7036219
_publ_section_title
;
 The first example of erbium triple-stranded helicates displaying SMM
 behaviour.
;
_journal_issue                   38
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              16833
_journal_page_last               16839
_journal_paper_doi               10.1039/c5dt02554k
_journal_volume                  44
_journal_year                    2015
_chemical_formula_moiety         'C84 H87 Er2 N24 O3, 3(N O3)'
_chemical_formula_sum            'C84 H87 Er2 N27 O12'
_chemical_formula_weight         2001.32
_space_group_crystal_system      trigonal
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2015-07-22 deposited with the CCDC.
2015-08-19 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            12
_cell_length_a                   26.1100(7)
_cell_length_b                   26.1100(7)
_cell_length_c                   48.0953(13)
_cell_measurement_reflns_used    8313
_cell_measurement_temperature    100(1)
_cell_measurement_theta_max      27.9890
_cell_measurement_theta_min      3.3110
_cell_volume                     28395.3(13)
_computing_cell_refinement       'CrysAlis Pro (Agilent Technologies (2011))'
_computing_data_collection       'CrysAlis Pro (Agilent Technologies (2011))'
_computing_data_reduction        'CrysAlis Pro (Agilent Technologies (2011))'
_computing_molecular_graphics    'Mercury (MacRae et al., 2009)'
_computing_publication_material  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SIR92 (Altomare et al., 1993)'
_diffrn_ambient_temperature      100(1)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 16.1544
_diffrn_detector_type            Eos
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Eos'
_diffrn_measurement_method       \w-scan
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0167
_diffrn_reflns_av_unetI/netI     0.0188
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       31
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -27
_diffrn_reflns_limit_l_max       57
_diffrn_reflns_limit_l_min       -36
_diffrn_reflns_number            17425
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        24.997
_diffrn_reflns_theta_max         24.997
_diffrn_reflns_theta_min         2.924
_exptl_absorpt_coefficient_mu    1.832
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.86336
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            pale-green
_exptl_crystal_density_diffrn    1.404
_exptl_crystal_description       prism
_exptl_crystal_F_000             12144
_exptl_crystal_preparation       'Magnetic properties'
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.15
_refine_diff_density_max         1.051
_refine_diff_density_min         -1.196
_refine_diff_density_rms         0.106
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.286
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     381
_refine_ls_number_reflns         5547
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.286
_refine_ls_R_factor_all          0.0563
_refine_ls_R_factor_gt           0.0392
_refine_ls_shift/su_max          0.028
_refine_ls_shift/su_mean         0.006
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0976P)^2^+3.8970P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1521
_refine_ls_wR_factor_ref         0.1660
_reflns_Friedel_coverage         0.000
_reflns_number_gt                4227
_reflns_number_total             5547
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c5dt02554k3.cif
_cod_data_source_block           4
_cod_depositor_comments
'Adding full bibliography for 7036214--7036219.cif.'
_cod_original_cell_volume        28395.3(17)
_cod_database_code               7036219
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              90917
_shelx_fab_checksum              48769